## Abstract

The combination of magnetic symmetries and electronic band topology provides a promising route for realizing topologically nontrivial quasiparticles, and the manipulation of magnetic structures may enable the switching between topological phases, with the potential for achieving functional physical properties. Here, we report measurements of the electrical resistivity of EuCd_{2}As_{2} under pressure, which show an intriguing insulating dome at pressures between *p*_{c1} ~ 1.0 GPa and *p*_{c2} ~ 2.0 GPa, situated between two regimes with metallic transport. The insulating state can be fully suppressed by a small magnetic field, leading to a colossal negative magnetoresistance on the order of 10^{5}%, accessible via a modest field of ~ 0.2 T. First-principles calculations reveal that the dramatic evolution of the resistivity under pressure can be attributed to consecutive transitions of EuCd_{2}As_{2} from a magnetic topological insulator to a trivial insulator, and then to a Weyl semimetal, with the latter resulting from a pressure-induced change in the magnetic ground state. Similarly, the colossal magnetoresistance results from a field-induced polarization of the magnetic moments, transforming EuCd_{2}As_{2} from a trivial insulator to a Weyl semimetal. These findings underscore weak exchange couplings and weak magnetic anisotropy as ingredients for discovering tunable magnetic topological materials with desirable functionalities.

## Introduction

Whereas the electronic band topology in nonmagnetic topological materials is determined by the crystal symmetry and the relative strength of spin-orbit coupling, the magnetic ground state also plays a decisive role in magnetic topological materials^{1,2,3,4,5,6,7}. The concurrence of magnetism and electronic band topology leads to unusual states of matter, including Weyl fermions in centrosymmetric systems^{8,9}, magnetic topological insulators^{10}, quantum anomalous Hall states^{11}, and axion insulators^{12}. The dependence of band topology on the magnetic ground state grants access to topological phase transitions by manipulation of the latter, and opens up a route for discovering functional properties in magnetic topological materials.

*f*-electron materials provide a fertile setting for discovering emergent physics at the intersection of magnetism, electron correlations and topology, including magnetic topological insulators^{13,14,15,16}, as well as topological spin textures^{17,18,19,20} and strongly correlated topological phases such as topological Kondo insulators and semimetals^{21,22,23,24}. Among the *f*-electron magnetic topological materials, EuCd_{2}As_{2}, which crystallizes into the trigonal CaAl_{2}Si_{2}-type structure^{25}, exhibits a single Dirac cone at the Fermi level well inside the paramagnetic state, offering an ideal platform for realizing exotic quasiparticles^{13,26,27}. Below the antiferromagnetic transition temperature *T*_{N} ≈ 9 K, the Eu^{2+} moments are oriented in the *a**b*-plane and form A-type antiferromagnetic (AFM) order, with antiferromagnetically stacked ferromagnetic (FM) Eu^{2+} layers^{28}. With such a magnetic ground state, a gap opens at the Dirac point and the system may be a small-gap magnetic topological insulator (MTI)^{14,29}. A fully polarized state along the *c*-axis can be readily obtained upon applying a magnetic field, giving rise to an ideal single pair of Weyl points^{14,30}. A Weyl state is also suggested for the paramagnetic phase slightly above *T*_{N} based on photoemission measurements, resulting from a proliferation of quasi-static in-plane ferromagnetic fluctuations^{31,32}. A plethora of additional topological states, including magnetic Dirac semimetals, axion insulator, and higher-order topological insulator, are also expected given the appropriate magnetic ground state^{29}. Moreover, in addition to becoming fully polarized under modest in-plane or *c*-axis magnetic fields^{28}, a FM ground state can be stabilized by changes in the synthesis protocol^{33} or applying hydrostatic pressure^{34}, demonstrating highly-tunable magnetism. These behaviors highlight the proximity of competing magnetic ground states in EuCd_{2}As_{2}, which can be harnessed to manipulate its electronic topology.

Here, by carrying out resistivity measurements on EuCd_{2}As_{2} single crystals under hydrostatic pressure, we find an insulating dome within a small pressure window between *p*_{c1} ~ 1.0 GPa and *p*_{c2} ~ 2.0 GPa, straddled by two regimes (*p* < *p*_{c1} and *p* > *p*_{c2}) with metallic transport. The insulating state is easily suppressed by a magnetic field (0.2 T for **H** ⊥*c*), leading to a remarkable colossal negative magnetoresistance (MR) which reaches ~10^{5}% at 0.3 K, and can likely be enhanced upon further cooling. Based on first-principles calculations, these experimental observations may arise from two topological phase transitions tuned by magnetism. Namely, a transition from an AFM topological insulator to an AFM trivial insulator (TrI) at *p*_{c1} ~ 1.0 GPa, and a transition from an AFM TrI to a FM Weyl semimetal (WSM) at *p*_{c2} ~ 2.0 GPa, triggered by a pressure-induced AFM-FM transition of the magnetic ground state. A similar mechanism accounts for the suppression of the TrI state under applied magnetic field, which polarizes the AFM state and transforms the system to a WSM, leading to the colossal MR. These findings demonstrate that the combination of Dirac fermions and proximate magnetic ground states provides a route for discovering tunable topological quantum materials with functional properties.

## Results

### Metallic-insulating-metallic evolution of electrical transport under pressure

EuCd_{2}As_{2} crystallizes in a centrosymmetric trigonal structure (space group \(P\bar{3}m1\)^{25}), with planes of Eu^{2+} that form triangular lattices [inset of Fig. 1a] separated by layers of Cd-As tetrahedra networks^{25}. Whereas the FM alignment of magnetic moments within the *a**b*-plane is robust, the stacking of these FM planes can be tuned between AFM or FM order along the *c*-axis, resulting in an overall A-type AFM or FM ground state^{28,33,35}. Given the proximity between these magnetic ground states, the physical properties of our EuCd_{2}As_{2} samples were carefully characterized at ambient pressure, with the results summarized in Fig. 1. Clear peaks in both the resistivity *ρ*(*T*) and specific heat *C*_{p}(*T*) are observed around *T*_{N} ≈ 9 K (Fig. 1a, b). Measurements of the magnetic susceptibility under a small field of 0.1 T (Fig. 1c) suggest an AFM ground state with an easy *a**b*-plane, in agreement with resonant x-ray scattering measurements^{28}. Magnetization measurements reveal saturation fields (saturated moments) of about 1.7 T (7.1 *μ*_{B}/Eu) for **H** ∥*c* and 0.7 T (7.0 *μ*_{B}/Eu) for **H** ⊥*c* (Fig. 1d). The saturated moments are close to the ideal value of 7.0 *μ*_{B} for Eu^{2+} ions, indicating localized magnetism. These characterizations establish that the EuCd_{2}As_{2} samples used in this study exhibit an A-type AFM ground state below *T*_{N} ≈ 9 K at ambient pressure, similar to previous reports^{28,34,36}.

In order to track the pressure-evolution of the ground state properties of EuCd_{2}As_{2}, electrical resistivity measurements were carried out on four samples under pressures up to 2.50 GPa and temperatures down to 0.3 K. The results for two samples #1 and #2 are presented in Fig. 2, and the others are shown in the Supplementary Fig. 1. All samples exhibit consistent behaviors under pressure.

For pressures up to 0.87 GPa (Fig. 2a, b), *ρ*(*T*) is qualitatively similar to that at ambient pressure, with a sharp peak around *T*_{N} and metallic behavior at low temperatures [*ρ*(0.3K) ≲ 20 mΩ ⋅ cm]. Upon increasing the pressure to 1.05 GPa, an additional subtle upturn appears when cooling below ~ 2 K. The upturn in *ρ*(*T*) at low temperatures becomes more prominent under 1.28 GPa, and is maximized around 1.50 GPa (Fig. 2c, d), with *ρ*(0.3K) reaching ≈ 40 Ω ⋅ cm and ≈15 Ω ⋅ cm, for samples #1 and #2 respectively [0 T data in Fig. 3e, f). The temperature-dependence of the resistivity under 1.50 GPa can be captured by \((\rho (T)-{\rho }_{0})\propto \exp (\frac{{{\Delta }}}{{k}_{{{{\rm{B}}}}}T})\), where *ρ*_{0} is a temperature-independent contribution and Δ represents an energy gap [insets in Fig. 2c, d]. This indicates that the upturn is associated with an electronic gap, suggesting a metal-insulator transition in EuCd_{2}As_{2} across *p*_{c1} ~1.0 GPa. By fitting *ρ*(*T*) of all measured samples for *T* < 5 K, Δ is consistently found to be ≈ 0.07−0.10 meV at 1.50 GPa (see Supplementary Fig. 1 and Supplementary Note 1), suggesting that Δ does not exhibit a significant variation in samples used in this work. We note that an insulating behavior in *ρ*(*T*) was not reported in Ref. ^{34} at 1.57 GPa down to 5 K, possibly related to signatures of the insulating state being weak at 5 K and sample differences.

Upon further increasing the pressure, the upturn in *ρ*(*T*) weakens under 1.79 GPa and disappears for *p* ≳ 2.21 GPa, at which *ρ*(0.3K) reverts back to ≲ 20 mΩ ⋅ cm. Such an evolution points to the restoration of metallic transport above *p*_{c2} ~ 2.0 GPa, and experimentally establishes the presence of an insulating dome within the magnetically ordered state for *p*_{c1} < *p* < *p*_{c2}. Since A-type AFM order is present in EuCd_{2}As_{2} up to ~ *p*_{c2}, as indicated by the response of the resistivity to small magnetic fields (see Supplementary Fig. 2 and Supplementary Note 2) and previous transport and *μ*SR measurements^{34}, the insulating state appears tied to the AFM order.

### Colossal magnetoresistance in the insulating state

To further elucidate the connection between the magnetic order and the insulating state under pressure, magnetoresistance measurements were carried out under 1.50 GPa for samples #1 and #2, and the results are shown in Fig. 3. Since the saturation field of EuCd_{2}As_{2} is small (Fig. 1d), and further reduces with increasing pressure^{34}, it is straightforward to assume that the A-type AFM order of EuCd_{2}As_{2} can be polarized to achieve a FM state using accessible magnetic fields. If the insulating state indeed relies on the presence of A-type AFM order, it should be suppressed when the AFM state becomes fully polarized.

At 1.5 GPa, with increasing field both along the *c*-axis and in the *a**b*-plane, *ρ*(0.3K) reduces by around three orders of magnitude, and settles to values less than 20 mΩ ⋅ cm, as shown in Fig. 3a, b. This transformation from insulating to metallic electrical transport is similar to the pressure-induced evolution across *p*_{c2}. Quantitatively, the MR [defined as [*ρ*(*H*) − *ρ*(0)]/*ρ*(0)] at 0.3 K reaches −3.78 × 10^{5}% for sample #1 with **H** ∥*c* [Fig. 3(c)], and −1.05 × 10^{5}% for sample #2 with **H** ⊥*c* (Fig. 3d). The values of the MR in EuCd_{2}As_{2} are large even when compared to the colossal MR in the manganites^{37,38,39}, and are even more striking considering that they are achieved with relatively small fields [caption of Fig. 3]. The fields at which the MR saturates are *μ*_{0}*H* ~ 1.5 T for **H** ∥*c* and *μ*_{0}*H* ~ 0.2 T for **H** ⊥ *c*, which are in excellent agreement with the saturation fields^{34}, and indicates that the MR is associated with polarization of the Eu^{2+} moments. At higher temperatures, the resistivity in zero field is substantially reduced, whereas the resistivity under \(\left|{\mu }_{0}H\right|\gtrsim 2\) T remains similar to that at 0.3 K. This leads to a weakening of the MR upon warming, originating from a decrease in the zero-field resistivity with increasing temperature.

The colossal negative MR can also be seen from the temperature dependence of the resistivity under various fields for samples #1 and #2 at 1.50 GPa, as shown in Fig. 3e, f. Similar to the results in Fig. 2c, d, where the insulating state is suppressed by increasing pressure above *p*_{c2}, modest magnetic fields also efficiently suppress the insulating state. In both cases, the A-type AFM phase is destabilized and superseded by a FM state, respectively due to an AFM-FM transition at *p*_{c2} ~ 2.0 GPa, or the full polarization of Eu^{2+} moments by an applied field. While a sizable MR is also seen in EuCd_{2}As_{2} at ambient pressure near *T*_{N}, it should be emphasized that the colossal MR we have uncovered in the insulating state of EuCd_{2}As_{2} is distinct. Whereas the former is associated with critical fluctuations near a magnetic transition with similar behaviors detected in a number of Eu-based compounds^{40,41,42}, the MR shown in Fig. 3 is linked to a field-induced transition from an insulating state with a small electronic gap Δ to a metallic state, and persists down to at least 0.3 K. Therefore, although the MR in our measurements may contain contributions related to critical fluctuations near the magnetic transition temperature, the MR at low temperatures (e.g. *T* < 2 K) clearly has a different, and thus far unreported mechanism.

From Fig. 3e, f, it can be seen that the low-temperature MR gradually decreases with increasing temperature. On the flip side, this suggests that the MR should continue to increase as the temperature is lowered below 0.3 K. In fact, since the resistivity tends to infinity for an insulator when the temperature approaches absolute zero, the MR could become substantially larger (possibly by orders of magnitude) than what we observed at 0.3 K. This consideration makes the colossal negative MR in EuCd_{2}As_{2} of potential interest for ultra-low-temperature applications, especially ones at millikelvin temperatures.

### Evolution of the electronic structure under pressure

The experimentally observed insulating dome is difficult to understand without considering magnetic order, and the colossal MR points to a strong coupling between electrical transport, which is dictated by the electronic topology, and magnetism. To gain insight into the origin of these experimental observations, the electronic structures of EuCd_{2}As_{2} were calculated for different magnetic ground states and at various pressures, using density functional theory (DFT), with results shown in Fig. 4. Applied pressures in DFT calculations are gauged via the unit cell volume *V*, with increasing pressure corresponding to a decrease in *V* (see Supplementary Note 3 and Supplementary Table 1). For the A-type AFM state with moments in the *a**b*-plane found experimentally^{28}, EuCd_{2}As_{2} is a MTI with a 10 meV bulk gap and topologically-protected surface states when *V* = 127.60 Å^{3} (Fig. 4a), and parity of the band states at time-reversal invariant momenta further indicate it can be categorized as an axion insulator (see Supplementary Note 3 and Supplementary Table 2). While the bulk of a MTI is insulating, topologically-protected surface states that cross the Fermi level [inset in Fig. 4a] give rise to metallic conduction, which accounts for the metallic conduction seen experimentally for *p* < *p*_{c1}.

Within the A-type AFM state of EuCd_{2}As_{2}, upon increasing pressure such that *V* = 124.78 Å^{3}, EuCd_{2}As_{2} evolves to become a TrI with an 8 meV trivial band gap (Fig. 4b), where relative to the MTI state, topologically-protected surface states disappear due to an increase in the electronic hopping relative to spin-orbit coupling, which suppresses band inversion. When *V* becomes further compressed from 124.78 Å^{3} to 121.11 Å^{3}, the trivial band gap increases from 8 meV to 64 meV (Fig. 4c). For a trivial insulator, its surface states are also gapped [insets in Fig. 4b, c], similar to the bulk, so that the system as a whole lacks mobile carriers. These calculations show that within the A-type AFM state of EuCd_{2}As_{2}, the transition from a MTI to a TrI upon increasing pressure provides an explanation for the experimentally observed evolution of electrical transport across *p*_{c1}.

While AFM EuCd_{2}As_{2} with *V* = 121.11 Å^{3} is a TrI [Fig. 4(c)], for a FM ground state with in-plane moments under the same pressure (same *V*), EuCd_{2}As_{2} is a WSM with bulk Weyl points and a surface Fermi arc [Fig. 4d and its inset]. Such a FM state occurs experimentally when the moments are fully polarized by an *a**b*-plane field or when *p* > *p*_{c2}, with both the Weyl points and the Fermi arc contributing to metallic transport. A FM state with moments along the *c*-axis is also a WSM for *V* = 121.11 Å^{3} (see Supplementary Note 3 and Supplementary Fig. 3), which is realized in the fully polarized state when **H** ∥*c*. The DFT results in Fig. 4c, d indicate that for AFM EuCd_{2}As_{2} in the TrI state, altering the magnetic order to FM results in a WSM, which induces a insulator-metal transition. Experimentally, such a change can occur in two ways, either by applying a magnetic field to fully polarize the moments (Fig. 3), or by increasing pressure above *p*_{c2} (Fig. 2c, d), around which an AFM-FM transition occurs (see Supplementary Fig. 2 and Supplementary Note 2)^{34}.

Based on the DFT calculations shown in Fig. 4, the evolution of the topological classification for EuCd_{2}As_{2} under pressure is schematically shown in Fig. 5a. Under ambient pressure and inside the AFM state, EuCd_{2}As_{2} is a small-gap MTI, with topologically-protected surface states contributing to metallic conduction. With increasing pressure, the bulk band inversion necessary for a topological insulator is suppressed and AFM EuCd_{2}As_{2} becomes a TrI, with diminished charge carriers when cooled to sufficiently low temperatures. When EuCd_{2}As_{2} goes through an AFM-FM transition, the TrI state evolves to become a WSM, with metallic conduction restored by Weyl fermions and surface Fermi arcs.

## Discussion

Our resistivity measurements under pressure provide compelling evidence for an unusual insulating dome inside the AFM state of EuCd_{2}As_{2} for pressures between *p*_{c1} ~ 1.0 GPa and *p*_{c2} ~ 2.0 GPa, with an AFM-FM transition in the magnetic ground state also occurring around *p*_{c2} (Fig. 5b). Such an evolution under pressure can be qualitatively captured by the DFT calculations, which suggest that EuCd_{2}As_{2} goes through consecutive topological phase transitions. Within this scenario, the first transition is from a MTI to a TrI at *p*_{c1}, occurring within the A-type AFM phase; the second transition that occurs at *p*_{c2} is from a TrI to a WSM, driven by the AFM-FM transition in the magnetic ground state. Given the proximity between the AFM and FM ground states^{35}, the AFM-FM transition can also be driven by an applied field, which accounts for the colossal MR achievable with a small magnetic field. In such a situation, similar to increasing pressure above *p*_{2}, the MR is caused by a change from a TrI to a WSM, which occurs both when FM moments are oriented along the *c*-axis or in the *a**b*-plane (see Supplementary Note 3, Supplementary Table 3, and Supplementary Figs. 3–6).

The colossal negative MR observed in EuCd_{2}As_{2} for *p*_{c1} < *p* < *p*_{c2} is unusual, as its magnitude is large, persists to the lowest temperatures, and likely arises from a field-induced topological phase transition from a TrI to a topologically nontrivial WSM. Given that the MR arises from an insulator-metal transition, record-breaking values of MR may be achieved upon cooling to ever lower temperatures. The small fields required to achieve the large values of MR further makes EuCd_{2}As_{2} appealing for technological applications at very low temperatures. The observation of colossal MR for small fields both along the *c*-axis and in the *a**b*-plane (Fig. 3c, d) means that the colossal MR would be robust regardless of the sample orientation, and would persist even in polycrystalline samples. While a modest pressure is required to access the TrI phase of EuCd_{2}As_{2} with the colossal MR, it may be possible to replace the hydrostatic pressure with chemical pressure via partial substitution of P for As, and realize a similar colossal MR under ambient pressure.

Whereas the transition from a MTI to TrI under pressure within the AFM state of EuCd_{2}As_{2} arises from enhanced electronic hopping that suppresses the band inversion, both the pressure- and field-induced transitions from a TrI to a WSM requires a transformation of the magnetic ground state. To facilitate such a change, the distinct magnetic ground states should be nearly degenerate, which in the case of EuCd_{2}As_{2} results from weak magnetic exchange couplings along the *c*-axis, which can be easily overcome by an applied magnetic field. Furthermore, EuCd_{2}As_{2} exhibits weak magnetic anisotropy due to the vanishing orbital moments of the Eu^{2+} ions, which allows the magnetic moments to become fully polarized regardless of the field orientation, leading to a robust colossal MR that is nearly independent of the relative orientation between the sample and the applied field. In combination with an electronic topology that depends on the magnetic structure, the weak interlayer magnetic exchange couplings and magnetic anisotropy in EuCd_{2}As_{2} enables the switching between magnetic ground states, and hence the electronic topology, leading to dramatic changes in the macroscopic electrical transport. These findings demonstrate a clear example of topological phase transitions driven by the manipulation of the magnetic ground state, and underscore weak magnetic exchange couplings and magnetic anisotropy as key ingredients in the search for tunable magnetic topological materials.

## Methods

### Experimental details

Single crystals of EuCd_{2}As_{2} were grown using the Sn-flux method, with synthesis details and basic characterizations in Refs. ^{43,44}. Electrical resistivity measurements under pressure were carried out in a piston-cylinder pressure cell using the standard four probe method, with the current in the *a**b*-plane. To ensure hydrostaticity, Daphne 7373 was used as the pressure-transmitting medium. Values of the applied pressure were determined from the shift of the superconducting transition temperature *T*_{c} for a high-quality Pb single crystal. All the resistivity measurements were performed down to 0.3 K in a ^{3}He refrigerator with a 15 T magnet. Specific heat under ambient pressure was measured using a Quantum Design Physical Property Measurement System (PPMS), using a standard pulse relaxation method. Magnetization measurements were carried out using the vibrating sample magnetometer (VSM) option in a Quantum Design PPMS.

### First-principles electronic structure calculations

The electronic structures of EuCd_{2}As_{2} under pressure were calculated from first principles using density functional theory (DFT). The DFT calculations were performed using the plane-wave projected augmented wave method as implemented in the VASP code^{45,46}. The Perdew, Burke and Ernzerho parameterization (PBE) of the general gradient approximation (GGA) was used for the exchange-correlation functionals^{47}. The plane-wave basis energy cut-off was set to 480 eV, and a 12 × 12 × 4 Γ-centered *k*-mesh was used to perform integration over the Brillouin zone. An additional on-site Coloumb interaction of *U* = 6 eV was included for the Eu-4*f* orbitals in the LDA+*U* calculations. Both the lattice constants and the atomic internal coordinates were optimized for all magnetic configurations, so that forces on each atom were smaller than 0.01 eV/Å. The band structures from VASP were fit to tight-binding Hamiltonians using the maximally projected Wannier function method. The resulting tight-binding Wannier-orbital-based Hamiltonians were used to calculate the corresponding surface states^{48} and analyze their electronic topology with the WannierTools package^{49}.

## Data availability

All data needed to evaluate the conclusions in the paper are present in the paper and/or the Supplementary Information.

## References

Tokura, Y., Yasuda, K. & Tsukazaki, A. Magnetic topological insulators.

*Nat. Rev. Phys.***1**, 126–143 (2019).Zou, J., He, Z. & Xu, G. The study of magnetic topological semimetals by first principles calculations.

*Npj Comput. Mater.***5**, 96 (2019).Kruthoff, J., de Boer, J., van Wezel, J., Kane, C. L. & Slager, R.-J. Topological classification of crystalline insulators through band structure combinatorics.

*Phys. Rev. X***7**, 041069 (2017).Watanabe, H., Po, H. C. & Vishwanath, A. Structure and topology of band structures in the 1651 magnetic space groups.

*Sci. Adv.***4**, eaat8685 (2018).Xu, Y. et al. High-throughput calculations of magnetic topological materials.

*Nature***586**, 702–707 (2020).Elcoro, L. et al. Magnetic topological quantum chemistry.

*Nat. Commun.***12**, 5965 (2021).Tang, F. & Wan, X. Exhaustive construction of effective models in 1651 magnetic space groups.

*Phys. Rev. B***104**, 085137 (2021).Kuroda, K. et al. Evidence for magnetic Weyl fermions in a correlated metal.

*Nat. Mater.***16**, 1090–1095 (2017).Liu, E. et al. Giant anomalous Hall effect in a ferromagnetic kagome-lattice semimetal.

*Nat. Phys.***14**, 1125–1131 (2018).Otrokov, M. M. et al. Prediction and observation of an antiferromagnetic topological insulator.

*Nature***576**, 416–422 (2019).Deng, Y. et al. Quantum anomalous Hall effect in intrinsic magnetic topological insulator MnBi

_{2}Te_{4}.*Science***367**, 895–900 (2020).Sekine, A. & Nomura, K. Axion electrodynamics in topological materials.

*J. Appl. Phys.***129**, 141101 (2021).Hua, G. et al. Dirac semimetal in type-IV magnetic space groups.

*Phys. Rev. B***98**, 201116 (2018).Wang, L.-L. et al. Single pair of Weyl fermions in the half-metallic semimetal EuCd

_{2}As_{2}.*Phys. Rev. B***99**, 245147 (2019).Xu, Y., Song, Z., Wang, Z., Weng, H. & Dai, X. Higher-order topology of the axion insulator EuIn

_{2}As_{2}.*Phys. Rev. Lett.***122**, 256402 (2019).Li, H. et al. Dirac surface states in intrinsic magnetic topological insulators EuSn

_{2}As_{2}and MnBi_{2n}Te_{3n+1}.*Phys. Rev. X.***9**, 041039 (2019).Kurumaji, T. et al. Skyrmion lattice with a giant topological Hall effect in a frustrated triangular-lattice magnet.

*Science***365**, 914–918 (2019).Hirschberger, M. et al. Skyrmion phase and competing magnetic orders on a breathing kagomé lattice.

*Nat. Commun.***10**, 5831 (2019).Kaneko, K. et al. Unique helical magnetic order and field-induced phase in trillium lattice antiferromagnet EuPtSi.

*J. Phys. Soc. Jpn.***88**, 013702 (2019).Puphal, P. et al. Topological magnetic phase in the candidate Weyl semimetal CeAlGe.

*Phys. Rev. Lett.***124**, 017202 (2020).Dzero, M., Sun, K., Galitski, V. & Coleman, P. Topological Kondo insulators.

*Phys. Rev. Lett.***104**, 106408 (2010).Kim, D. J. et al. Surface Hall effect and nonlocal transport in SmB

_{6}: evidence for surface conduction.*Sci. Rep.***3**, 3150 (2013).Xu, N. et al. Direct observation of the spin texture in SmB

_{6}as evidence of the topological Kondo insulator.*Nat. Commun.***5**, 4566 (2014).Guo, C. Y. et al. Evidence for Weyl fermions in a canonical heavy-fermion semimetal YbPtBi.

*Nat. Commun.***9**, 4622 (2018).Artmann, A., Mewis, A., Roepke, M. & Michels, G. AM

_{2}X_{2}-verbindungen mit CaAl_{2}Si_{2}-struktur. XI. struktur und eigenschaften der Verbindungen ACd_{2}X_{2}(A: Eu, Yb; X: P, As, Sb).*Z. Anorg. Allg. Chem.***622**, 679–682 (1996).Niu, C., Mao, N., Hu, X., Huang, B. & Dai, Y. Quantum anomalous Hall effect and gate-controllable topological phase transition in layered EuCd

_{2}As_{2}.*Phys. Rev. B***99**, 235119 (2019).Xu, Y. et al. Unconventional transverse transport above and below the magnetic transition temperature in Weyl semimetal EuCd

_{2}As_{2}.*Phys. Rev. Lett.***126**, 076602 (2021).Rahn, M. C. et al. Coupling of magnetic order and charge transport in the candidate dirac semimetal EuCd

_{2}As_{2}.*Phys. Rev. B***97**, 214422 (2018).Ma, J. et al. Emergence of nontrivial low-energy Dirac fermions in antiferromagnetic EuCd

_{2}As_{2}.*Adv. Mater.***32**, 1907565 (2020).Soh, J.-R. et al. Ideal Weyl semimetal induced by magnetic exchange.

*Phys. Rev. B***100**, 201102 (2019).Ma, J.-Z. et al. Spin fluctuation induced Weyl semimetal state in the paramagnetic phase of EuCd

_{2}As_{2}.*Sci. Adv.***5**, eaaw4718 (2019).Soh, J.-R. et al. Resonant x-ray scattering study of diffuse magnetic scattering from the topological semimetals EuCd

_{2}As_{2}and EuCd_{2}Sb_{2}.*Phys. Rev. B***102**, 014408 (2020).Jo, N. H. et al. Manipulating magnetism in the topological semimetal EuCd

_{2}As_{2}.*Phys. Rev. B***101**, 140402 (2020).Gati, E. et al. Pressure-induced ferromagnetism in the topological semimetal EuCd

_{2}As_{2}.*Phys. Rev. B***104**, 155124 (2021).Krishna, J., Nautiyal, T. & Maitra, T. First-principles study of electronic structure, transport, and optical properties of EuCd

_{2}As_{2}.*Phys. Rev. B***98**, 125110 (2018).Wang, H. P., Wu, D. S., Shi, Y. G. & Wang, N. L. Anisotropic transport and optical spectroscopy study on antiferromagnetic triangular lattice EuCd

_{2}As_{2}: an interplay between magnetism and charge transport properties.*Phys. Rev. B***94**, 045112 (2016).von Helmolt, R., Wecker, J., Holzapfel, B., Schultz, L. & Samwer, K. Giant negative magnetoresistance in perovskitelike La

_{2/3}Ba_{1/3}MnO_{x}ferromagnetic films.*Phys. Rev. Lett.***71**, 2331–2333 (1993).Jin, S. et al. Thousandfold change in resistivity in magnetoresistive La-Ca-Mn-O films.

*Science***264**, 413–415 (1994).Salamon, M. B. & Jaime, M. The physics of manganites: structure and transport.

*Rev. Mod. Phys.***73**, 583–628 (2001).Oliver, M. R., Dimmock, J. O., McWhorter, A. L. & Reed, T. B. Conductivity studies in Europium oxide.

*Phys. Rev. B***5**, 1078–1098 (1972).Shapira, Y. & Reed, T. B. Resistivity and Hall effect of EuS in fields up to 140 kOe.

*Phys. Rev. B***5**, 4877–4890 (1972).Wang, Z.-C. et al. Colossal magnetoresistance without mixed valence in a layered Phosphide crystal.

*Adv. Mater.***33**, 2005755 (2021).Sun, Y. et al. Experimental evidence for field-induced metamagnetic transition of EuCd

_{2}As_{2}.*J. Rare Earths*(in press). https://doi.org/10.1016/j.jre.2021.08.002 (2021).Wang, Y. et al. Long-time magnetic relaxation in antiferromagnetic topological material EuCd

_{2}As_{2}.*Chin. Phys. Lett.***38**, 077201 (2021).Kresse, G. & Hafner, J. Ab initio molecular dynamics for liquid metals.

*Phys. Rev. B***47**, 558–561 (1993).Kresse, G. & Joubert, D. From ultrasoft pseudopotentials to the projector augmented-wave method.

*Phys. Rev. B***59**, 1758–1775 (1999).Perdew, J. P., Burke, K. & Ernzerhof, M. Generalized gradient approximation made simple.

*Phys. Rev. Lett.***77**, 3865–3868 (1996).Sancho, M. P. L., Sancho, J. M. L., Sancho, J. M. L. & Rubio, J. Highly convergent schemes for the calculation of bulk and surface green functions.

*J. Phys., F. Met. Phys.***15**, 851–858 (1985).Wu, Q., Zhang, S., Song, H.-F., Troyer, M. & Soluyanov, A. A. Wanniertools: an open-source software package for novel topological materials.

*Comput. Phys. Commun.***224**, 405–416 (2018).

## Acknowledgements

We acknowledge helpful discussions with Zhentao Wang, Wei Zhu, and Yang Liu. This work was supported by the National Key R&D Program of China (No. 2017YFA0303100), the National Natural Science Foundation of China (No. 11974306, No. 12034017 and No. 11874137), and the Key R&D Program of Zhejiang Province, China (2021C01002).

## Author information

### Authors and Affiliations

### Contributions

F.D., L.Y., Z.N., S.L., Y.C. and D.S. carried out the experimental measurements. Y.L. and Y.Shi prepared the samples. F.D., N.W. and C.C performed the first-principles calculations. L.Y. initiated this study and H.Y. supervised the project. F.D., C.C., Y.Song and H.Y. analyzed the results. Y.Song, H.Y., C.C., M.S., and F.S. wrote the manuscript, with input from all authors.

### Corresponding authors

## Ethics declarations

### Competing interests

The authors declare no competing interests.

## Additional information

**Publisher’s note** Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.

## Supplementary information

## Rights and permissions

**Open Access** This article is licensed under a Creative Commons Attribution 4.0 International License, which permits use, sharing, adaptation, distribution and reproduction in any medium or format, as long as you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in a credit line to the material. If material is not included in the article’s Creative Commons license and your intended use is not permitted by statutory regulation or exceeds the permitted use, you will need to obtain permission directly from the copyright holder. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0/.

## About this article

### Cite this article

Du, F., Yang, L., Nie, Z. *et al.* Consecutive topological phase transitions and colossal magnetoresistance in a magnetic topological semimetal.
*npj Quantum Mater.* **7**, 65 (2022). https://doi.org/10.1038/s41535-022-00468-0

Received:

Accepted:

Published:

DOI: https://doi.org/10.1038/s41535-022-00468-0